International Research Journal of Engineering and Technology (IRJET) Volume: 03 Issue: 07  July2016
eISSN: 2395 0056 pISSN: 23950072
www.irjet.net
OPTIMIZATION OF PROCESS PARAMETERS IN TURNING OF ALUMINIUM METAL MATRIX COMPOSITES K.Ramadevi1, Dr.R.Ramachandra2, Dr.D.SaiChaithanya Kishore3,B.Sreenivasulu4 1, M.Tech student, department of mechanical engineering, S.K.D engg. college, Gooty. 2, Principal, department of mechanical engineering, S.K.D engg.college, Gooty. 3, associate professor, department of mechanical engineering, KL university, vaddeswar 4, associate professor & HOD, department of mechanical engineering, S.K.D engg.college, Gooty. ***adding precision rotational features to a part whose basic shape has already been formed.
Abstract  This paper investigates the study of mechanical and machining behavior of Aluminium 7075with (0, 2.5, 5 wt%) of TiB2 and TiC. The insitu composite was prepared by liquid metallurgy route. The composite was prepared with the formation of the reinforcement inside the molten matrix by adding salts of Potassium Tetra fluoro borate (KBF4), graphite and Potassium Hexa fluoro titanate (K2TiF6). Turning is carried out on a lathe machine that provides the power to turn the work piece at a given rotational speed and to feed the cutting tool at a specified rate and depth of cut therefore, three cutting parameters, i.e. cutting speed, feed rate, and depth of cut, need to be determined in a turning operation.MRR and CF are important parameters to evaluate cutting performance. The influence of cutting speed, feed rate depth of cut and percentage reinforcement is examined. The model for the MRR and CF, is obtained using DOE in MINITAB16. The main objective of this paper is to carry out the experiments by selecting different variables and their levels, applying TAGUCHI and ANOVA, and then analyzing the results obtained. The results obtained conclude that TAGUCHI and ANOVA is reliable methods and it can be readily applied to different metal cutting processes with greater confidence. The mechanical properties in terms of hardness and impact test were carried out. It was observed that the hardness and impact strength of Al70755% TiB2 & TiC insitu composite was improved by the Al7075 alloy respectively. Key Words: Optimization; turning; Taguchi; Anova; MRR; Cutting force.
Fig.1. turning operation in lathe machine Taguchi method is used for find a specific range and combinations of turning parameters like cutting speed, feed rate and depth of cut to achieve optimal values of response variables like Cutting force, material removal rate in turning of aluminium hybrid material material. ANOVA is used to investigate the process parameters which significantly affect the performance characteristics. Aluminum7075 have the chemical composition of different materials with percentages are indicated in below table: 1 Table1: Chemical composition of Al7075 alloy Al7075
Al
Cu
Mg
Si
Cr
Fe
Mn
Zn
Mtrl.%
89.20
1.76
2.55
0.10
0.19
0.25
0.09
5.81
1. INTRODUCTION Metal Matrix composites (MMCs) are the combination of two or more distinct phases that has improved properties than the monolithic alloy. The application of MMCâ€™s greatly increasing due to their high strength and toughness at elevated temperatures coupled with lowdensity.
2. EXPERIMENTAL SETUP 2.1: Fabrication of Al7075TiCTiB2 Fabrication of Al70752.5wt% of TiC & TiB2 was carried out in a batch of 3 kg of Al and 2.5 wt% TiC & TiB 2. the reinforcement was carried out by 240.72 grams of K2TiF6 (Potassium hexa fluoro titanate) and 15.6 grams of graphite powder was used for the formation of TiC, and
Turning is also commonly used as a secondary process to add or refine features on parts that were manufactured using a different process. Due to the high tolerances and surface finishes that turning can offer, it is ideal for
ÂŠ 2016, IRJET

Impact Factor value: 4.45

ISO 9001:2008 Certified Journal

Page 753
International Research Journal of Engineering and Technology (IRJET) Volume: 03 Issue: 07  July2016
www.irjet.net
240.72 grams of K2TiF6 (Potassium hexa fluoro titanate) and 240.72 grams of KBF4 was used for the formation of TiB2 . Al7075 was melted in crucible and premixed K2TiF6, KBF4 and graphite powder of measured quantity were added to the molten aluminium.
removal rate (MRR). The process parameters with three levels of cutting speed, feed and depth of cut were used for the optimization study and a list of process parameters were displayed in below. Table 2: process parameters and their levels
Stir casting process starts with placing empty crucible in the muffle. At first heater temperature is set to 500°C and then it is gradually increased up to 900°C. The molten material was held for 30 minutes and the melt was stirred at regular intervals during this exothermal reaction will take place between the molten aluminium and halide salt K2TiF6. The reaction between the salt (K2TiF6) and molten aluminium releases Ti, the solute Ti reacts with C to produce TiC particles, and the KBF4 reacts with Al release B2 this combines with Ti forms TiB2 happens by holding the melt for 30 minutes. After 30 minutes the slag is removed from the molten mix and the molten mix is poured into the cast iron mould, shown in fig. Similarly Al70755 wt%TiCTiB2 was fabricated by using proper ratios of K2TiF6, KBF4 and C.
1
315
0.13
0.25
0
500
0.34
0.5
2.5
0.75
5
775
0.55
3.1: EXPERIMENTAL DESING Experiments are conducted based on planned design, the Three spindle speeds (N) 315 rpm, 500 rpm, and 775 rpm. Three feed rates (f) 0.13 mm/rev, 0.34 mm/rev, and 0.55 mm/rev. Three depth of cuts (d) 0.25mm,0.5mm, and 0.75mm.three different percentage reinforcements 0%,2.5% and 5% were selected. Details of experimental design, control factors and their levels, results for MRR and Cutting forces are shown in table 4.4. these tables show that the experimental plan had three levels and four parameters.
3.2: TAGUCHI DESIGN A standard Taguchi experimental plan with notation L27 was chosen. The rows in the L27 orthogonal array used in the experiment denotes each trial and the columns contained the factors to be studied. The first column consisted of spindle speed, the second contained feed, and the third column contained depth of cut consecutive column consisted of the Percentage of reinforcement. In the Taguchi method, the experimental results are transformed into a signaltonoise (S/N) ratio. This method recommends the use of S/N ratio to measure the quality characteristics deviating from the desired values. To obtain optimal testing parameters, thehigherisbetter quality characteristic for machining the metal was taken
2.2: TURNING OPERATION Turning operation is carried out in a Lathe Machine manually under an operator’s supervision. There are two types of motion in a turning operation. One is the cutting motion which is the circular motion of the work and the other is the feed motion which is the linear motion given to the tool. The three machining parameters i.e., Spindle speed, Feed rate and Depth of cut are used for material removal rate.
due to measurement of the MRR. The S/N ratio for each level of testing parameters was computed based on the S/N analysis. With S/N ratio analysis, the optimal combination of the testing parameters could be determined
3. EXPERIMENTAL INVESTIGATION There are various responses considered during turning of AlTic/TIB2 MMCs, all these responses were optimized by using Taguchi method. Taguchi method is best technique to select the best parameter combination for to get best minimized and maximized response value. Taguchi method is applied separately for each individual response output. The response output considered for the Taguchi optimization study are Cutting force (CF) and material
Impact Factor value: 4.45
%Reinforcem ent
Speed (rpm)
3
The work piece rotates in the lathe, with a certain spindle speed (N), at a certain number of revolutions per minute. The power measurements are made with the help of a wattmeter.

Process parameters Feed Rate Depth Of (mm/rev) Cut(mm)
Level
2
Fig:2 Casting Process
© 2016, IRJET
eISSN: 2395 0056 pISSN: 23950072
TABLE3: Signal To Noise Ratio For Mrr and Cf

ISO 9001:2008 Certified Journal

Page 754
International Research Journal of Engineering and Technology (IRJET) Volume: 03 Issue: 07  July2016
www.irjet.net
It could be seen in Table: 4 that the strongest influence was exerted by Feed rate, followed by Depth of cut, spindle speed, and lastly percentage reinforcement. Since the first level of the Material removal rate was about 67.64 mm/rev while the third level of the Material removal rate was about 79.47mm/rev the difference being the most highest of 11.83 mm/rev. It is followed by the Depth of cut which is 9.38mm which is significant level again. Which is followed by the spindle speed with 5.57rpm and The reinforcement showed the least effect on the Material removal rate which is 0.51.
S/N ratio
E X P
Speed (rpm)
Feed (mm/ rev)
Doc (mm)
% R
MRR (mm3/ min)
S/N ratio
CF (N)
1
315
0.13
0.25
0
956
59.9
0.037
29.13
2
315
0.13
0.5
2.5
1897
65.5
0.038
28.24
3
315
0.13
0.75
5
2822
68.8
0.041
26.80
4
315
0.34
0.25
0
2460
67.9
0.034
29.20
5
315
0.34
0.5
2.5
4794
73.5
0.036
28.31
6
315
0.34
0.75
5
7002
76.8
0.045
26.87
7
315
0.55
0.25
0
3911
71.7
0.041
28.46
8
315
0.55
0.5
2.5
7483
77.3
0.039
27.57
9
315
0.55
0.75
5
10715
80.6
0.050
26.13
10
500
0.13
0.25
2.5
1365
62.8
0.031
30.39
11
500
0.13
0.5
5
2552
68.2
0.030
30.12
12
500
0.13
0.75
0
4249
72.3
0.029
30.22
13
500
0.34
0.25
2.5
3504
70.8
0.029
30.45
14
500
0.34
0.5
5
6408
76.2
0.034
30.19
15
500
0.34
0.75
0
10514
80.3
0.030
30.28
16
500
0.55
0.25
2.5
5561
74.6
0.029
29.71
17
500
0.55
0.5
5
9934
80.0
0.037
29.45
18
500
0.55
0.75
0
16036
84.2
0.032
29.54
19
775
0.13
0.25
5
1760
65.0
0.028
31.75
20 21 22 23 24 25 26 27
775 775 775 775 775 775 775 775
0.13 0.13 0.34 0.34 0.34 0.55 0.55 0.55
0.5 0.75 0.25 0.5 0.75 0.25 0.5 0.75
0 2.5 5 0 2.5 5 0 2.5
3718 5519 4501 9312 13503 7113 14394 20337
71.2 74.7 73.0 79.3 82.7 76.8 83.1 86.5
0.022 0.026 0.025 0.021 0.029 0.022 0.023 0.037
33.02 30.95 31.81 33.08 31.02 31.07 32.34 30.27
eISSN: 2395 0056 pISSN: 23950072
CHART1: Effects Of Means For S/N Ratio
The signaltonoise ratio for the biggerthebetter is CHART2: Effects Of Means Of Means Where
CHART 2 shows the main effect plots for Material removal rate of the metal for S/N ratios. Optimal testing conditions of these control factors could be very easily determined from the response graph. The best Material removal rate value was at the higher S/N value in the response graph. For main control factors indicates the optimum condition for the tested samples (A3, B3, C3, D1). Thus, it could be concluded that the maximum Material removal rate of metal is achieved and their optimal setting of control factors for tested samples are shown in Table3.
i= Experiment number u= Trail number Ni= Numberof trails for experiment I TABLE4: Response Table For Signal To Noise Ratios Larger is better Level
Speed (rpm)
Feed (mm/rev)
Doc (mm)
%R
1
71.38
67.64
69.20
74.48
2 3 Delta
74.43 76.95 5.57
75.65 79.47 11.83
74.98 78.58 9.38
74.31 73.97 0.51
Rank
3
1
2
4
To obtain optimal testing parameters, thelowerisbetter quality characteristic for machining the metals was taken due to measurement of the Cutting force. The SignalToNoise ratio for the SmallerTheBetter is
Where
ÂŠ 2016, IRJET

Impact Factor value: 4.45

ISO 9001:2008 Certified Journal

Page 755
International Research Journal of Engineering and Technology (IRJET) Volume: 03 Issue: 07  July2016
www.irjet.net
i= Experiment number u= Trail number Ni= Numberof trails for experiment i
Analysis of variance is a mathematical technique which is based on the least square approach. The purpose of ANOVA is to investigate the process parameters which significantly affect the performance characteristics. As per this technique, if the calculated value of the F ratio of the developed model does not exceed the standard tabulated value of F ratio for a desired level of confidence, then the model is considered to be adequate within the confidence limit. The variance ratio, denoted by F in ANOVA tables, is the ratio of the mean square due to a factor and the error mean square. In robust design, F ratio can be used for qualitative understanding of the relative factor effects. A high value of F means that the effect of that factor is large compared to the error variance. So, the larger the value of F, the more important is that factor in influencing the process response.
TABLE5: Response Table for Cutting force Smaller is better Level
Speed(rpm)
Feed(mm/rev)
Doc(mm)
%R
1 2 3 Delta Rank
27.86 30.04 31.70 3.85 1
30.07 30.13 29.39 0.74 4
30.22 30.26 29.12 1.14 3
30.59 29.66 29.35 1.23 2
eISSN: 2395 0056 pISSN: 23950072
It could be seen in Table: 5 that the strongest influence was exerted by spindle speed followed by percentage reinforcement, Depth of cut and lastly feed rate. Since the first level of the Cutting force was about 27.86 rpm while the third level of the Cutting force was about 31.7 rpm the difference being the most highest of 3.85 rpm. It is followed by the percentage reinforcement with 1.23, which is significant level again. Which is followed by the Depth of cut, about 1.14 and The feed rate showed the least effect on the Cutting force was 0.74.
Table6: Results Of Anova For Mrr Source
Adj SS
Adj MS
FValue
Speed
D F 2
80786493
40393246
11.27
Feed
2
277522636
138761318
38.73
Doc
2
197113163
98556581
27.51
%R
2
10718222
5359111
1.50
Error
1 8 2 6
64486412
3582578
Total
630626925
Table7: ANOVA For The Response Mrr SOURC E SPEED FEED D.O.C %R ERROR TOTAL
CHART3: Effects Of Means For S/N Ratio
DO F 2 2 2 2 18 26
SQUARES SUM 80786479 2.78E+08 1.97E+08 10718222 64485526 6.31E+08
MEAN OF SQUARE 40393240 1. 39E+08 98556707 5359111 3582529
F RATIO 11.2750 38.7328 27.5103 1.49590
% OF CONTRIB UTION 12.81050 44.00752 31.25673 1.699613 10.2256
The results of the ANOVA of Material removal rate in turning of work piece are shown in Table 6. In addition to degree of freedom, mean of squares (MS), sum of squares (SS) and Fratio associated with each factor level were presented. This analysis was performed for a confidence level of 90%. The F value for each design parameters was calculated. The calculated value of the F showed a high influence of the feed rate (f) on the Material removal rate since Fcalculation was equal to 38.73, but the depth of cut (d), Spindle speed (N) and percentage reinforcement (%R) had also significant effects on the surface roughness since Ftest was equal to 27.51mm,11.27rpm and 1.50 respectively.
CHART4: Effects Of Means Of Means
3.3: ANALYSIS OF VARIANCE (ANOVA)
ÂŠ 2016, IRJET

Impact Factor value: 4.45

ISO 9001:2008 Certified Journal

Page 756
International Research Journal of Engineering and Technology (IRJET) Volume: 03 Issue: 07  July2016
www.irjet.net
Table8: Analysis Of Variance For Cutting Force Source Speed
DF 2
Adj SS 0.000947
Adj MS 0.000474
FValue 56.48
feed Doc
2 2
0.000056 0.000114
0.000028 0.000057
3.36 6.31
%R Error
2 18
0.000106 0.000151
0.000053 0.000008
6.81
Total
26
0.001375
Rockwell hardness number is automatically indicated on the dial gauge or digital display. High Rockwell hardness numbers represent hard material sand low numbers soft materials. Table: 10 Rockwell Hardness Test
Table9: Anova For The Response Cutting Force MEAN OF SQUARE
SOURCE
DO F
SQUARE S SUM
SPEED
2
0.000947
0.000474
FEED
2
5.63E05
2.82E05
D.O.C
2
0.000114
5.72E05
%R Error TOTAL
2 18 26
0.000106 0.000151 0.001375
5.29E05 8.38E06
F RATIO 56.563245 82 3.3639618 14 6.3215990 45 6.8156324 58
% OF CONTRIBU TION 68.91088
8.317934
Load(Kgf)
Hardness(Hrb)
1 2
AL7075(0% of Tic & TiB2) AL7075(2.5% of Tic & TiB2)
100 100
74 76
3
AL7075(5% of Tic & TiB2)
100
83
The test specimen bar of 30mm diameter (d1) and 40mm length has to be the jaws of the universal testing machine. Close the inlet / outlet valves and switch on the machine. Apply the load slowly by opening the inlet valve. Noted the load when the pointer needle deflects (yield load –YL). Start increasing the load by opening the inlet valve. Note down the load when the bar breaks (ultimate tensile load – UTL). The final diameter (d2) and final length (L2) are measured by joining the two broken specimen. Calculate the yield & ultimate strength.
7.700982 10.97417
Table: 11 Tensile Test
The mathematical relationships between responses and machining parameters were established using multiple regression analysis. In the present study, the correlation between the process parameters cutting velocity, feed rate, depth of cut, MRR and CF are established. The multiple linear regression models were obtained using MINITAB 16.
Sl. No
Composites
UltimateTensil e Strength(Mpa)
Percentageo f Elongation (%)
1 2
AL7075(0% of Tic & TiB2) AL7075(2.5% of Tic & TiB2)
112 115
15 13
3
AL7075(5% of Tic & TiB2)
120
11
A significant improvement is observed in the tensile strength of the composite with increasing percentage reinforcement of material.
Regression equation for MRR + 18690 feed
4. CONCLUSION
Regression equation for CF
In Current work we will investigated and optimized Cutting parameters speed, feed and Depth Of Cut (DOC) for different proportions of Al7075 with (0 wt%,2.5 wt%,5 wt%) of TiCTiB2. From the Taguchi optimization study it was observed that the best parameter combination for to get higher MRR for turning is A3 (775rpm), B3 (0.55mm/rev), C3 (0.75mm) and D1(0 wt%) i.e., higher cutting speed, higher feed, higher depth of cut and lower percentage reinforcement, and the best parameter combination for to get lower cutting force is A1 (315rpm), B3
CF = 0.03957  0.000030 spindle speed + 0.00717 feed + 0.00896 doc + 0.000963 %R 3.5: ROCKWEEL HARDNESS TEST The minor load is applied first and a SET position is established on the dial gauge or displacement sensor of the Rockwell tester. Then the major load is applied. Without moving the piece being tested, the major load is removed and, with the minor load still applied, the

Composites
3.6: TENSILE TEST
4.101862
3.4: STATISTICAL ANALYSIS
© 2016, IRJET
Sl. No
A significant improvement is observed in the hardness of the composite with increasing percentage reinforcement of material and a decrease in the ductility.
The response values for MRR in ANOVA gives percentage contribution of each parameter shown in Table: 5.5.1. The feed contribution is highest which is 44%, followed by depth of cut is 31.2%, and spindle speed is 12.8% and lastly percentage reinforcement which is 1.69% and the error occurred in this is 10%.
MRR =10346 + 9.12 spindle speed + 13236 doc  283 %R
eISSN: 2395 0056 pISSN: 23950072
Impact Factor value: 4.45

ISO 9001:2008 Certified Journal

Page 757
International Research Journal of Engineering and Technology (IRJET) Volume: 03 Issue: 07  July2016
www.irjet.net
eISSN: 2395 0056 pISSN: 23950072
(0.55mm/rev), C3 (0.75) and D3 (5 wt%) i.e., lower cutting speed, higher feed, higher depth of cut and higher percentage reinforcement.
[7] Kalaiselvan, K., Murugan, N., Siva Parameswaran., 2011. Production and characterization of AA6061B4C stir cast composite. Materials and Design, 32, 40044009.
From The Analysis of variance (ANOVA) for material removal rate the strongest influence was exerted by Feed rate (44 mm/rev), followed by Depth of cut (31.2 mm), spindle speed (12.8 rpm), and lastly percentage reinforcement (1.69), and for cutting force the strongest influence was exerted by spindle speed (68.9 rpm), followed by Depth of cut (8.31 mm), percentage reinforcement (7.7 wt%) and lastly Feed rate (4.10 mm/rev).
[8] Kerti Isil., 2005. Production of TiC reinforced aluminium composites with the addition of elemental carbon. Mater Lett, 59, 37953800. [9] Lewis, D., 1991. InSitu Reinforcement of Metal Matrix Composites. Metal Matrix Composites: Processing and Interface, Academic Press London, 121150. [10] Mahamani, A., Anandakrishnan, V., 2010. Multiresponse optimization of turning parameters of Al6061TiB2 insitu metal matrix composite using greytaguchi method. International ejournal of mathematics and engineering, 246255.
A significant improvement is observed in the tensile strength and hardness of the composite with increasing percentage reinforcement of material, and a decrease in the ductility of the composite is observed with increasing percentage reinforcement of material. Hence in the future we can use this Hybrid composite Al7075TiCTiB2 to improve machining parameters, Strength and hardness in the automobile industry.
[11] Mahamani, A., 2011. Machinability Study of Al5CuTiB2 Insitu Metal Matrix Composites Fabricated by Fluxassisted Synthesis. Journal of Minerals & Materials Characterization & Engineering, Vol. 10, No. 13, 12431254. [12] Mahamani, A., Muthukrishnan, N., Anandakrishnan, V., 2012. Determination of optimum parameters for multiperformance characteristic in turning of Al 60616% ZrB2 insitu Metal Matrix Composite using grey relational analysis. International journal of manufacturing, materials and mechanical engineering, volume 2, issue 1.
REFERENCES [1] Sai Chaitanya Kishore, D., Prahlada Rao, K., Mahamani, A., 2013. Fabrication and characterisation of insitu AlTiC composite. International journal of mechanical engineering and technology, volume 4, issue 1, 109114.
[13] Pradeep Kumar Jha., Anand Kumar., Mahapatra, M, M., 2013. Influence of machining on Al4.5CuTiC InSitu Metal Matrix composites. Light metals, John Wiley & Sons, 449452.
[2] Mahamani, A., 2011. Mechanism of Insitu Reinforcement Formation in Fabrication of AA6061TiB2 Metal Matrix Composite. Indian foundry journal, Vol 57, No 3.
[14] Anandakrishnan, V., Mahamani, A., 2011. Investigations of flank wear, cutting force, and surface roughness in the machining of Al6061TiB2 in situ metal matrix composites produced by fluxassisted synthesis. Int J Adv Manuf Technnol, 55, 6573.
[3] Cui, C., Shen, Y., Meng, F., 2000. Review on Fabrication Methods of Insitu Metal Matrix Composites. Journal of Material Science Technology, Vol. 16, pp. 619626.
[15] Birol, Y., 2008. In situ synthesis of AlTiCp composites by reacting K2TiF6 and particulate graphite in molten aluminium. Journal of Alloys and Compounds, 454, 110117.
[4] Daniel, B, S, S., Murthy, V, S, R., Murty, G, S., 1997. Metal Ceramic Composites Via Insitu Methods. Journal of Materials Processing Technology, Vol. 68, pp.132155. [5] Jerome, S., Ravisankar, B., Pranab Kumar Mahato., Natarajan, S., 2006. Synthesis and evaluation of mechanical and high temperature tribological properties of insitu Alâ€“TiC composites. Material Science and Engineering, A 428, 3440.
Dr.R.Ramachandra received his Ph.D in Internal combustion engines from jntu Hyderabad. He is having total 20 years of Teaching and Research Experience and he is member in Professional bodies viz. Institute of Engineers and International Association of
[6] Kaczmar, J, W., Pietrzak, K., Wlosinski, W., 2000. The production and application of metal matrix composite materials. J Mater Process Technology, 106, 5867.
ÂŠ 2016, IRJET

Impact Factor value: 4.45
Engineers.

ISO 9001:2008 Certified Journal

Page 758
https://irjet.net/archives/V3/i7/IRJETV3I7144.pdf
Published on Mar 8, 2018
https://irjet.net/archives/V3/i7/IRJETV3I7144.pdf